This test procedure serves as a general purpose atmospheric corrosion test and can be applied to a wide variety of materials, coatings and interactions of materials. It has been developed to allow the evaluation of the corrosion resistance of metals in environments where there is a significant influence of chloride ions, mainly as sodium chloride from a marine source or by winter road de-icing salt. This test is cyclic in nature, i.e.; test specimens are exposed to changing climates over time.
Test specimens are placed in an enclosed chamber and exposed to a changing climate. The first 5 days comprise of the following 3 part repeating cycle. 6.0 hours exposure to a ‘wet’ climate of no less than 95% RH, at +25°C, with intermittent exposure to salt solution. This is followed by 2.5 hours climate controlled transition to 50°C & 70% RH. This is followed by 15.5 hours exposure to a constant climate of 50°C & 70% RH. The final 2 days comprise of 48.0 hours exposure to a constant climate of 50°C & 70% RH. This completes the total 7 day test cycle. The number of cycle repeats and therefore the test duration is variable.
This test is also referred to as a Cyclic Corrosion Test, often abbreviated to CCT.
Q-fog鹽霧試驗箱用于Volvo VCS 1027,1449鹽霧測試的流程
溫馨提醒：本Volvo VCS 1027,1449可能存在更新的版本，建議尋找Volvo VCS 1027,1449的發行商確認。
Q-FOG CCT1100鹽霧腐蝕試驗機具有1103升大容量測試能力，可在一臺機器中實現高濕度、干燥、靜止、加熱等多個不同的循環測試條件。Q-FOG CCT1100 馬上詢價
Q-FOG CRH1100是一款的具有相對濕度控制功能和溶液噴淋功能的鹽霧試驗箱.Q-FOG CRH1100 馬上詢價
Q-FOG CRH600比起SSP/CCT鹽霧試驗箱增加了一個可調濕度控制功能，這意味著CRH鹽霧試驗箱具備更廣泛的標準適用范圍。Q-FOG CRH600 馬上詢價
Q-LAB CCT600鹽霧腐蝕試驗箱不僅具備了SSP 鹽霧試驗箱的所有優點，同時還增加100%濕度功能。CCT600測試樣品容量為640升Q-FOG CCT600 馬上詢價